2 AN ABSTRACT OF THE THESIS OF Sidi Lian for the degree of Master of Science in Materials Science presented on December 19, Title: Heat Treatment Effects on CPM-M4 Tool Steel Performance as Edged Blade Material. Abstract approved: Julie Tucker CPM-M4 tool steel is a commonly used knife blade material due to its high strength and wear resistance. The goal of this thesis is to understand how heat treatment parameters affect blade performance and microstructure. Five heat treatments were applied to CPM-M4 steel by varying austenitizing and tempering temperatures. The microstructures were examined by optical microscopy, scanning electron microscopy and limited amounts of energy-dispersive X-ray spectroscopy. The carbide fraction, size, count, spacing and chemistry were characterized from the microstructural analysis. Blade performance was examined by hardness, 3-Point bend, impact, and CATRA (edge retention) testing. The results show that the austenitizing temperature is a significant factor that affects all mechanical properties tested. The max load in 3-Point bend test increases with the carbides fraction that can be maximized by controlling austenitizing temperature. Both austenitizing temperature and tempering temperature have significant effects on the hardness. As for the impact performance, the impact toughness increases with
3 the carbides density. Additionally, we can achieve comparatively high impact toughness in low austenitizing temperature without decreasing hardness through lowering the tempering temperature, because tempering temperature has no significant effect on impact toughness. The edge retention of CPM-M4 steel relates to its hardness. Harder materials can provide a better edge retention for knife blade.
4 Copyright by Sidi Lian December 19, 2014 All Rights Reserved
5 HEAT TREATMENT EFFECTS ON CPM-M4 TOOL STEEL PERFORMANCE AS EDGED BLADE MATERIAL by Sidi Lian A THESIS submitted to Oregon State University in partial fulfillment of the requirements for the degree of Master of Science Presented December 19, 2014 Commencement June 2015
6 Master of Science thesis of Sidi Lian presented on December 19, 2014 APPROVED: Major Professor, representing Materials Science Director of the Materials Science Program Dean of the Graduate School I understand that my thesis will become part of the permanent collection of Oregon State University libraries. My signature below authorizes release of my thesis to any reader upon request. Sidi Lian, Author
7 ACKNOWLEDGEMENTS The author expresses sincere appreciation to Dr. Julie Tucker for her support and guidance as advisor, Dr. David Kim and Dr. Hector Vergara for their support as project advisors and contributions in this study, and Martin Mills, Gary Schuster and Dave Maxey for their technical support. The author would also like to express personal appreciation to Bjorn Westman, Zach Terrell and Cody Fast.
8 TABLE OF CONTENTS Page 1 INTRODUCTION REVIEW OF LITERATURE INTRODUCTION POWDER METALLURGY CCT DIAGRAM OF M4 STEEL HEAT TREATMENT PRACTICE WEAR-RESISTANCE SUMMARY EXPERIMENT DESIGN OBJECTIVES AND REQUIREMENTS OF THE EXPERIMENT HEAT TREATMENT PARAMETERS EXPERIMENT EXECUTION SAMPLE PREPARATION FOR MICROSTRUCTURE EXAMINATION Introduction Standard Preparation Procedures PROCEDURES OF MICROSTRUCTURE ANALYSIS Introduction Procedures PROCEDURES OF EDGED BLADE PERFORMANCE TESTS Introduction Procedures RESULTS MICROSTRUCTURE: EDGE PERFORMANCE... 43
9 TABLE OF CONTENTS (Continued) Page Hardness Test Point Bend test Impact test CATRA test SUMMARY OF RESULTS DISCUSSION CONCLUSION FUTURE WORK BIBLIOGRAPHY APPENDICES LIST OF ABBREVIATIONS LIST OF SYMBOLS STANDARD SAMPLE PREPARATION PROCEDURES ANOVA TABLES... 81
10 LIST OF FIGURES Figure Page Figure 1. The continuous cooling transformation diagram for AISI M4 tool steel ...6 Figure 2. CCT diagram for M4 steel austenitized at 1220 C ... 8 Figure 3. Objectives of experiment design...17 Figure 4. The effect of tempering temperature and time for M4 steel  Figure 5. Summary of sample preparation procedure Figure 6. Rockwell hardness tester...28 Figure 7. Five hardness readings...28 Figure 8. Impact test machine Figure 9. 3-Point Bend test machine Figure 10. CATRA test machine...32 Figure 11. Optical microstructure of CPM-M4 steel, austenitized at 2100 F, tempered at 1025 F, magnification is 500X...34 Figure 12. Phase identification of CPM-M4 steel, autenitized at 2200 F, tempered at 925 F Figure 13. Chemical composition of the Mo,W-rich carbides (upper) and the V-rich carbides (below) from EDX analysis...36 Figure 14. Comparison of carbides fraction and size among heat treatments.38 Figure 15. SEM images of different heat treatment samples (a-e represent A-T-, A-T+, Center, A+T-, A+T+, respectively)...40 Figure 16. Comparison of carbides count and interparticle spacing among different heat treatments...42 Figure 17. Comparison of hardness among different heat treatments...44 Figure 18. Max load in 3-Point Bend test comparison among different heat treatments Figure 19. Impact results comparison among different heat treatments Figure 20. CATRA test results for different heat treatments... 49
11 LIST OF FIGURES (Continued) Figure Page Figure 21. CATRA results comparison among different heat treatments...51 Figure 22. Comparison of carbides fraction and max load in 3-Point bend test for different heat treatments Figure 23. Comparison of hardness results with carbides fraction and carbides size...58 Figure 24. Comparison of impact toughness with austenitizing temperature and carbides fraction Figure 25. Comparison of impact test results with carbides count Figure 26. Comparison of cutting edge retention results with carbides fraction...62 Figure 27. Comparison of cutting edge retention results and hardness...63 Figure 28. Comparison of edge performance...67
12 LIST OF TABLES Table Page Table 1. Chemical composition of CPM-M4 steel (in weight percent)... 2 Table 2. Heat treatment controlling matrix for CPM-M4 steel...19 Table 3. Average carbides fraction and size of different heat treatments Table 4. Carbides count and interparticle spacing for different heat treatments Table 5. Hardness results of different heat treatment samples...43 Table 6. 3-Point Bend results for different heat treatment samples Table 7. Impact test results for different heat treatment samples...47 Table 8. CATRA test results for different heat treatment samples Table 9. Summary of edge performance test results and microstructure analysis... 52
13 LIST OF APPENDIX FIGURES Figure Page Figure 29. SEM specimen section...75 Figure 30. SIMPLIMET II machine used for mounting fabrication Figure 31. Chill block used for cooling...78 Figure 32. Specimen with a final mount Figure 33. Grinding table Figure 34. Rotation polishing wheel... 79
14 LIST OF APPENDIX TABLES Table Page Table 10. ANOVA table for carbides size Table 11.ANOVA table for carbides fraction Table 12. ANOVA table for carbides count...82 Table 13. ANOVA table for interparticle spacing Table 14. ANOVA table for hardness test Table 15. ANOVA table for 3-Point Bend test Table 16. ANOVA table for impact test...84 Table 17. ANOVA table for comparison between average carbides sizes of the center heat treatment and the responding as-quenched sample...84 Table 18. ANOVA table for operator comparison in the hardness test... 84
15 LIST OF EQUATIONS Equation Page Equation 1. Formula for Rockwell Hardness C numbers ...28 Equation 2. Formula for determining impact energy...46 Equation 3. Formula of diffusion coefficient...53
16 1 HEAT TREATMENT EFFECTS ON CPM-M4 TOOL STEEL PERFORMANCE AS EDGED BLADE MATERIAL 1 INTRODUCTION The purpose of this project is to understand the effects of heat treatment parameters on the microstructure and performance of steel knife blades. Understanding this relationship will allow for the optimization of knife properties. Several characteristics of knife blades influence their performance, including cutting edge geometry, bevel geometry, blade profile, and the properties of the parent material, such as hardness, toughness and wear-resistance. Heat treatments are critical for improving the properties of the parent material. Different heat treatment parameters will result in different properties of the base materials. The heat treatment process must be optimized to achieve the best combination of properties for a given application. This work explores the role of austenitizing and tempering temperatures on knife blade performance for alloy CPM-M4. CPM-M4 is a high speed tool steel produced by powder-metallurgy. CPM-M4 has high vanadium, molybdenum and tungsten content, which provide good wear-resistance and cutting edge stability . M4 is also known for having a good combination of hardness and toughness. The chemical composition of CPM-M4 used in this study and the AISI-M4 composition are shown in Table 1.
17 2 Table 1. Chemical composition of CPM-M4 steel (in weight percent) C Cr Mn Mo P S Si V W Fe CPM-M4* Bal. 9 3 AISI-M Max 0.03 Max Bal. *Independent chemical analysis ASTM standards E and E A series heat treatments are performed in order to optimize CPM-M4 for knife blade performance. Austenitizing, quenching and tempering are the three major steps of the heat treatment process. There are many parameters that can be controlled for each of these steps including temperature, time and media. Austenitizing is a high temperature heat treatment performed to transform the room temperature microstructure (ferrite+pearlite) to austenite. During this phase transformation, carbides are dissolved and distributed in the austenite matrix. Following austenization, the material is rapidly cooled (quenching) to transform the matrix into martensite, which is a hard, brittle phase. Toughness is returned to the material by tempering at an intermediate temperature. During tempering the martensite phase is transformed into tempered martensite and carbides can nucleate and grow. In this study, the austenitizing and tempering temperature were varied while all other parameters were held constant. The resulting microstructure of the heat treated steels was examined by Optical Microscopy, Scanning Electron Microscopy (SEM) and Energy-dispersive X-ray spectroscopy (EDX). The average size, distribution and fraction of carbides were analyzed by statistical methods and the alloy content of different phases was defined by element analysis.
18 3 Differences in microstructures will affect knife blade performance. In order to correlate microstructure to mechanical properties, several tests were performed including: Rockwell C hardness test, 3-point bend fracture toughness test, impact toughness test, and CATRA cutting edge stability test. The results from mechanical testing and microstructure examination help relate heat treating parameters to the knife blade performance. This understanding will guide future heat treatments to fully optimize M4 in this application. The rest of the thesis is organized as follows: Chapter 2 introduces the background through the literature review. Chapter 3 describes the experiment design of this study. In Chapter 4, the experiment execution is described, including the procedures of the microstructure analysis and the performance tests. The results are presented in Chapter 5, then a discussion of the results is given in Chapter 6. Chapter 7 and 8 state the conclusions drawn from this study and the possible future work.
19 4 2 REVIEW OF LITERATURE 2.1 INTRODUCTION In this chapter, the background of the Powder-Metallurgy process is presented first, to explain how the process changes the material s properties and microstructure. Then, the literature based on the continuous cooling transformation (CCT) diagram of M4 steel is reviewed to describe the heat treatment processes. Next, the basic principles of heat treatment processes are presented and recommended heat treatment practices are discussed. Finally, the wear-resistance of M4 steel is discussed. 2.2 POWDER METALLURGY In addition to adjusting alloy content and applying specific heat treatments to improve steels, different manufacturing techniques are employed to lower cost and improve performance. Powder metallurgy (PM) is one of these techniques that is applied in CPM-M4 steel. PM is an alternative method of producing steel, it is based on compacting the metal powder into specific shapes under high temperature and pressure , . The PM process provides fine carbide sizes and uniform carbides distribution resulting in good dimensional stability and toughness. Humans have thousands of years of experience in the PM method, which can be traced back to ancient Egypt . From the second half of the 20 th century, PM has been a popular and important method in modern steel industry. As for practical applications of PM, Randall M. German (1998) introduced two
20 5 extreme methods in his book . One method is to densify the metal powders in sintering, while the other is a pressing process. In industry, different companies apply their own processes between these two extremes . The PM method has many advantages. It is easier to shape materials into more complex components with PM as compared to traditional methods. Additionally, the PM process also makes the microstructure of the final product more controllable, which usually provides a fine and uniform carbides distribution. Therefore, PM methods have been a popular practice in modern steel manufacturing. To achieve optimal performance of CPM-M4, a proper selection of heat treatment parameters is required. In this study, we will focus on the effect of heat treatment on mechanical properties. The relationship between specific heat treatments and the resulting microstructures will be analyzed. The continuous cooling transformation (CCT) diagram is a useful tool for selecting heat treatment parameters. 2.3 CCT DIAGRAM OF M4 STEEL From a data sheet of Erasteel Company , a rough CCT diagram shows the martensite transformation start temperature ( M s temperature) at around 300 F (150 C). The CCT diagram is presented in Figure 1. The general areas of austenite, bainite, pearlite and martensite are shown in the diagram.
21 6 Figure 1. The continuous cooling transformation diagram for AISI M4 tool steel  To develop a more accurate CCT diagram for M4 steel, Briki (2007)  performed a study based on the new evolution of the dilatometric method. In recent years, the dilatometric method has been improved significantly, which provides a more sensitive and precise way to detect the transformation during the cooling process of even some minor transformations . In their experiment, M4 steel was austenitized at 2228 F, than cooled at different cooling rates from F/s to 392 F/s. Two dilatometers, DI24 and DT1000 were used to detect the dimensional changes in the experiment. By using scanning electron microscopy and energy-spectrum analysis, the microstructure showed the gray color V-rich carbides with size of 10-15µm and the white color W-rich carbides with size of 1-5µm before austenitizing. The M23C6 carbides were dissolved at 1922 F, while the M6C and MC carbides were dissolved at higher than 2228 F. Therefore, carbides would be partially dissolved during austenitizing at 2228 F.
22 7 Dilatometric curves under different cooling rates were plotted after the cooling process. Phase transformations can be determined by derivative curves. In fast cooling rate (greater than 59 F/s) condition, the Ms temperature was identified at 374 F and the Mf (martensite transformation finish) temperature at -130 F, when samples were cooled in liquid nitrogen. However, a quite low Mf temperature would lead to an incomplete martensite transformation with a large volume of retained austenite . In this case, there was about 15% retained austenite in as-quenched condition. In a medium cooling rate (from F/s to 59 F/s), a splitting phenomena happened that resulted in two Ms temperatures. The first Ms temperature ranges from 392 F to 788 F by decreasing the cooling rate from 59 F/s to F/s. The retained austenite was less for the fast cooling rate, since the Mf temperature was increased to a relative high temperature. When the cooling rate was slower than 33.8 F/s, the Mf temperature was detected at greater than 194 F. In a slow cooling rate (slower than F/s), bainite, pearlite and ferrite were formed instead of austenite-martensite transformation. The new CCT diagram for M4 steel is shown in Figure 2. According to their study about the M4 CCT diagram, a medium cooling rate should be applied to achieve less retained austenite and more carbides precipitation , , .
23 8 Figure 2. CCT diagram for M4 steel austenitized at 1220 C  On the basis of the CCT diagram for M4 steel and the specific properties needed for tool steels, some guidelines for heat treatment practices have been developed. The following section discusses the common heat treatment practices for M HEAT TREATMENT PRACTICE As a significant part of metallurgy, many studies have been performed in the area of steel heat treating. Generally, steel heat treatments consist of austenitizing, quenching and tempering. Each step plays its own role in developing the microstructure and properties of a steel, however, they can also affect or cooperate with each other. Austenite is a solid solution of carbon and alloy elements in γ-iron, which has the face-centered cubic (F.C.C.) crystal structure. The process of a plain carbon steel forming single-phase austenite, when heated above a critical
24 9 temperature for a long time, is called austenitizing . The austenite transformation temperature is where pure iron change from the body-centered cubic (B.C.C) crystal structure to F.C.C upon heating . Due to the F.C.C structure, austenite can accommodate a higher solubility of carbon. Krauss (1980) explained the better carbon solubility in F.C.C structure. In B.C.C and F.C.C crystal structures, there are two kinds of interstitial sites, octahedral and tetrahedral. In octahedral sites, there are 6 nearest neighbor atoms, and there are 4 for the tetrahedral site. According the lattice parameter and geometry in F.C.C austenite, an atom 0.052nm in radius can be accommodated in an octahedral site and an atom 0.028nm in radius can fill a tetrahedral site. However in ferrite, a B.C.C structure, the atom radius is only 0.019nm in octahedral site and 0.035nm in tetrahedral site. Obviously, the austenite structure can provide more room for carbon atoms in octahedral site, although some expansion is needed since the carbon atom have a radius of 0.07nm . In plain carbon steel, the austenitizing temperature ranges from 723 C to 1493 C according to the percentage of carbon content. It s a very large temperature range, so a proper temperature selection is important in this process. For high alloy steels, the increased amount of alloy elements form stable carbides, which need to be dissolved by increasing the austenitizing temperature . Thelning said that most alloy elements increase the austenite transformation temperature except some austenite-formers like Ni and Mn . More alloy elements dissolved in the matrix usually results in a more
25 10 uniform carbide distribution after tempering. For M4 steel, a relatively high austenitizing temperature should be applied because of its high alloy element contents. All of the alloy elements in M4, such as chromium, vanandium, molybdenum and tungsten, increase the austenitizing temperature. However, most of the alloy elements depress the start temperature martensite transformation when they dissolve in the iron matrix, which causes difficulty in the next process, quenching. A lower martensite start temperature will increase the higher content of austenite retained after quenching. Therefore, proper temperature selection is important for achieving specific properties . For M4 steel, most practices [1,2,11,12] recommend an austenitizing temperature in the range between 2150 F and 2250 F for cutting-tool application. In this temperature range, a relatively high tempered hardness, which is between 64.5 HRC to 67 HRC, can be achieved. In Crucible Datasheet , austenitizing between 1875 F-2125 F is recommended for cold-working tools. However, ZAPP Materials Engineering  gives its recommendation of 2080 F-2150 F as the austenitizing temperature for cutting-tools and 1950 F-2050 F for cold-working tools, which require a higher toughness. The other objective of the austenitizing process is to form martensite, which can only be produced from austenite. To achieve the martensite transformation, a quenching process should be applied following austenitizing. Martensite is a metastable phase formed when an extremely fast cooling rate is applied to the austenite phase. It preserves the carbon content of the original
26 11 austenite. So it can be considered as ferrite in a supersaturate condition . Therefore, the tetragonal distortion caused by the supersaturate carbon leads to a body-centered tetragonal (B.C.T) crystal structure of martensite. Because of the B.C.T structure, martensite has much higher hardness than any other phases. Te is the metastable equilibrium temperature for martensite. However, a lower temperature is required to provide enough driving force for the martensite transformation. This temperature is also called martensite transformation start temperature, Ms . The final temperature in the quenching process should reach to at least Ms. To get a full transformation, another critical temperature, Mf (martensite finish), should be reached. However, there also retains some austenite content even when the cooling reach to Mf. Obviously, determining the Ms and Mf temperatures is extremely important in the quenching process. Generally, the Ms and Mf temperatures depend on the alloy elements in the steel. Most of alloy elements decrease both Ms and Mf temperatures [2,14]. To avoid forming other phases such like bainite and pearlite, the cooling rate should be kept as fast as possible in the quenching process. However, the cooling rate is usually limited to the possible distortion or cracking during the transformation. To some extent, the additional alloy elements can deal with this problem. That means that the high-alloy steel can bear a faster cooling rate, which could lead to a fully martensite transformation.
27 12 Quenching media also plays an important role. A proper media can provide a stronger and uniform driving force that will affect the microstructure and the mechanical properties of the final product. In general, salt bath or oil quenching to 1000 F then air quenching to below 125 F is stated in most of the datasheets for M4 steel. For small materials, air quenching to 125 F directly is also reasonable. However, it cannot be applied on large materials, because it cannot provide a uniform cooling rate and may lead to distortion or cracking [1,12,13]. Although martensite is hard, it is not a desirable material in most manufacture applications because, a low ductility accompanies the high hardness. As knife steel, martensite is too fragile to be selected as the final structure. As Wilson  stated in his book: as-quenched martensite should never be in the final structure. A tempering process will help to soften the martensite by removing the tetragonal distortion and facilitating the precipitation of carbides. Tempering at different temperatures will result in different stages of the phase transformation and different properties will be achieved. Let s assume the tempering temperature starts from 32 F. At the beginning, the hardness will be increased slightly due to the formation of some thin carbide plate . A maximum hardness will be achieved at 212 F for plain carbon steel accompanying with the formation of ε carbides. However, Madeleine also mentioned the temperature range for these carbides as 122 F-320 F . Generally, tempering below 482 F will lead to a good combination of hardness and toughness, due to the offset of increasing hardness by carbides
28 13 precipitation and increasing toughness by transforming martensite to tempered-martensite. When the temperature stays between 482 F-752 F, the modification of tetragonal distortion will be increased significantly and lead to a significant drop in hardness. However, toughness cannot be increased significantly at this temperature range because a phenomenon called 500 F temper brittleness. Wilson stated two reasons for this phenomenon. First reason is that the retained austenite-bainite transformation results in a loss of toughness, due to the brittleness of the bainite structure. Carbides also play an important role in this case. The carbides precipitate in grain boundaries making it more brittle . In this aspect, some metallurgists also mentioned that the formation of orthorhombic carbides, Fe3C is the reason of temper brittleness . After that, a significant drop in hardness and increase in toughness will happen when the temperature stays between 698 F-1247 F . Choosing the tempering temperature properly will decide what kind of properties are achieved in the final product. The alloying elements should be considered when deciding the tempering temperature. Most elements will retard the soften rate. That means a higher temperature is required when given properties should be achieved . At higher temperatures, the alloy carbides will substitute for the Fe3C carbides that usually leads to an increasing in hardness called secondary hardening . As for temper brittleness, to some extent, elements like molybdenum eliminate this phenomenon because they will not precipitate in grain boundaries as carbides.
29 14 Multiple tempering steps are required for M4 steel. The maximum hardness can be achieved at 980 F due to the secondary hardening [2, 11, 12]. For better toughness, tempering at 1000 F to 1100 F is most generally recommended [1,2, 11-13]. Although there are many heat treatment recommendations, the specific parameters should be selected by the specific properties required. For M4 steel, good wear-resistance is its characteristic mechanical property. Therefore, some research focusing on the wear-resistance of M4 had been studied and will be discussed in the next section. 2.5 WEAR-RESISTANCE Wear-resistance can be divided into two kinds of wear-resistance, adhesive and abrasive. M4 has excellent performance in both situations. To better understand wear performance, Fontalvo  performed a study to correlate the microstructure to the wear performance. In his study, carbides are the focus of the microstructural analysis. There were 6 alloys studied. M4 steel is the basic alloy, while the other 5 alloys have carbide content range from 0-25% in 5% increments. To keep the same composition and microstructure of the after-tempered martensite matrix, the compositions were simulated by the software Thermo-Calc and heat treatment parameters were decided by both Thermo-Calc and a dilatometer. Then, the only variable value is the carbides content and distribution. A Ball-on-Disk experiment was used in his study and the wear performances were compared with each other by using the volume of transfer materials. From the experiment results and microstructure analysis,
30 15 both carbides content and distance between carbides were concluded as the main parameters determining the adhesive wear performance. Higher carbides content and smaller distance between carbides can improve the adhesive wear performance . As for abrasive wear performance, Wang  also mentioned M4 in his study. D2 steel was selected as the reference material in this experiment. Five kinds of steel powders clad on the substrate materials, AISI 1070 carbon steel. M4 powder is one of them. A Falex dry sand wheel test machine was applied in the abrasive wear test. The mass loss was calculated to compare the abrasive wear resistance. After comparing the abrasive behavior and the analysis of microstructures, both carbides and matrix microstructures were confirmed as determining factors in abrasive wear resistance of these steels, including M4 steel. Although the Mo-rich and W-rich carbides in M4 steel were harder than the chromium carbides in D2 steel, the abrasive resistance of M4 was inferior to D2 due to the tiny size of Mo-rich and W-rich carbides. However, in the comparison between M4 and CPM 10V steel, CPM 10V had better abrasive behavior due to harder V-rich carbides and larger volume fraction of carbides content, although the carbides sizes are comparable between CPM 10V and M4 . 2.6 SUMMARY By reviewing of literature, we can clarify that a tempered-martensite matrix with fine size and uniform distributed carbides would be the desirable microstructure of CPM-M4 tool steel. According to the CCT diagram of M4
31 16 steel, a medium cooling rate (from F/s to 59 F/s) should be applied. The heat treatment practices are fairly common from different sources, austenitizing around 2100 F, air quenching to 125 F and multiple tempering steps between 1000 F and 1100 F are recommended. Excellent wear-resistance is a characteristic property of CPM-M4 steel. Higher carbides content and smaller carbide distances improve the adhesive wear performance . The carbides size and type affects the abrasive-wear resistance . From the studies discussed above, some relationships between microstructures and wear resistance were investigated. The other mechanical properties are just mentioned on their values or given a general explanation in most of the reviewed literature. There is a lack of studies based on specific heat treatments for M4 steel. Most articles in the literature just state recommendations. Some mention the relationships between heat treatment parameters and the mechanical properties. However, microstructure, the bridge between heat treatment and mechanical performance, should be investigated comprehensively, quantitatively and with a sound scientific method.
32 17 3 EXPERIMENT DESIGN 3.1 OBJECTIVES AND REQUIREMENTS OF THE EXPERIMENT The objective of this project is to relate heat treatment parameters to the microstructure and knife blade performance for CPM-M4 steel. The objectives of the experiment are shown schematically in Figure 3. The characteristic microstructure of the steel can be achieved by a specific heat treatment. Additionally, the edged blade performance also corresponds to the characteristic microstructure. Therefore, the microstructural analysis can be seen as a bridge in this study. To figure out how heat treatment affects the edged blade performance, the characteristic microstructure should be analyzed. Figure 3. Objectives of experiment design Controlling the heat treatment parameters is the key point in the experimental design. When a parameter is changed, all other parameters should remain
33 18 fixed, since different heat treatment parameters usually affect each other in the heat treatment process. Then the comparison between the heat treatments is based on a single parameter. As for the variation range, we will select a proper range according to two objectives. First, it should be in a reasonable range for austenitizing and tempering. For example, a good balance of hardness and toughness should be achieved for knife blade materials, so it s impractical if the tempering temperature is too low. On the other hand, to avoid the effects from uncontrollable factors, the parameters under control should achieve a significant difference in both the performance test and microstructure analysis. For the performance tests, each test should be kept consistent to avoid the effects from uncontrollable noise factors. A testing procedure should be standardized for each performance test. The standard testing procedures are shown in the later chapter. To decide which kind of performance should be tested, a functional principle should be applied. Only properties relating to the edged blade performance are to be tested in this study. The characteristic features of microstructure should be quantified. To get valid data and analysis results, the data collecting procedures should be kept consistent and the data analysis procedures should be appropriate. 3.2 HEAT TREATMENT PARAMETERS According to the objectives and requirements of the experimental design, the matrix of heat treatment parameters is shown in Table 2. Two parameters are controlled in the experiment, austenitizing temperature and tempering temperature. The parameters marked in red color represent the the center point
34 19 of the experiment design (austenitized at 2100 F and double tempered at 1025 F). Additionally, a higher and lower parameter are applied for both processes, which are 2000 F and 2200 F for austenitizing and 925 F and 1125 F for tempering. Then, four different heat treatments are selected by combining the two parameters for each of the two processes. The experimental design generates a 2x2 matrix with a center point. The corners make a set of single variable experiments while the center point helps to explain coupled effects. To achieve full carbides participation and retained austenite transformation, double-temper is applied for the tempering process. The double temper is denoted by (X2) in Table 2. Table 2. Heat treatment controlling matrix for CPM-M4 steel Aust Temp Temper Aust Temp Temper Aust Temp Temper ( F) Temp ( F) ( F) Temp ( F) ( F) Temp ( F) X X X X X 2 The austenitizing and tempering processes will affect both microstructure and material performance significantly. Temperature and time are the two factors for each process, which means the processes are easier to control and compare. Although quenching is also an important heat treatment process, it s much more complex to control. Many factors will affect the quenching process, such
35 20 as cooling rate, quenching media, sample dimensions and equipment. We use a consistent quenching process in our experiment. All of the heat treatment samples are quenched to below 125 F in nitrogen gas (at a medium quenching rate). Then the samples will be frozen at -120 F for 2 hours. The Ms temperature for M4 is between 392 F and 788 F and Mf temperature is around 194 F under a medium-cooling rate. Therefore the quenching process we use can achieve a full martensite transformation. The holding time of tempering and austenitizing is related to temperature. In general, lower temperatures need longer holding time to achieve similar performance. The effect of tempering time and temperature is shown in Figure 4 . Figure 4 shows the tempering temperature is more effective as compared to the holding time. For austenitizing, the time-temperature relationship is similar. The austenitizing process is less sensitive to time than to temperature. When the austenitizing temperature reaches a relatively high range, there is a negligible affect caused by changing the holding time. In this study, both austenitizing and tempering time are held constant, which are 30 minutes for austenitizing and 120 minutes for each of the double tempering processes.
36 21 Figure 4. The effect of tempering temperature and time for M4 steel  According to the literature and different datasheets for CPM-M4 steel heat treatments, austenitizing at 1950 F-2250 F is applicable for CPM-M4 steel. As for tempering temperature, 1000 F-1100 F are commonly recommended to balance hardness and toughness, which is a little higher than the secondary hardening temperature range (around 980 F). The center heat treatment in the experimental design (austenizing at 2100 F, temper at 1025 F) is in agreement with the recommendations from most of the reviewed literature. To generate a significant difference in microstructure and blade performance and still obtain practical properties for knife blade materials, ±100 F can be applied as a proper range of temperature change for both austenizing and tempering. In the following chapters, five different heat treatments will be represented by A-T-, A-T+, center, A+T-, A+T+. A represents austenitizing, T represents tempering, - represents lower temperature, + represents higher temperature, center represents the center heat treatment parameters.
37 22 The experiment will be executed to apply the five different heat treatments as shown in Table 2. Eighty (80) samples were heat treated at the same time for each heat treatment. To better understand the role of the two heat treatment processes on the microstructure, as-quenched samples were also prepared after the three austenitizing treatments (2000 F, 2100 F, 2200 F). For edge performance testing, hardness, toughness and cutting edge stability were selected as the representative properties of M4 steel. Also, the quantified microstructural analysis will focus on carbides fraction, size, count and distribution.
38 23 4 EXPERIMENT EXECUTION 4.1 SAMPLE PREPARATION FOR MICROSTRUCTURE EXAMINATION Introduction The first step in microstructural analysis is preparing the steel specimen so that distinct microstructure features (phases, grains) can be examined by both optical microscope and scanning electron microscope (SEM). Different materials require specific preparation procedures. Five heat treatments were applied on CPM-M4 steel in this study. However, they all have similar features such as high hardness, identical alloy composition, and after heat treating their microstructures consists of tempered martensite and a variety of carbides. Therefore, the same sample preparation procedure can be used with the different heat treatments specimens studied Standard Preparation Procedures Four procedures are applied to prepare specimens for SEM imaging: Sectioning, Mounting, Grinding and Polishing, and Etching (see details in Appendix 3). Figure 5 shows a summary of the different steps needed for specimen preparation for SEM imaging.
39 24 Figure 5. Summary of sample preparation procedure 4.2 PROCEDURES OF MICROSTRUCTURE ANALYSIS Introduction Microstructural analysis is an effective technique to indicate how heat treatments change the specific properties of the knife steels, since the properties changes will be reflected in the microstructures. To apply scientific analysis and get statistically-representative data, the procedures should be standardized to avoid noise factors during the experiment Procedures Microstructure examination by optical microscope Optical microscope is a reasonable technique for consistency examination. In this project, 500X is a proper magnification to get overall views of the microstructures of the samples. Three test coupons in the same dimension, 1 inch X 4 inches, were heat treated for each group (austenizing/tempering combination). Each test coupon was
40 25 prepared using our standard procedures (detailed in Appendix 3). Next, three optical images were taken in different areas on each sample. The optical images of each group were compared to examine the consistency between different coupons and areas. The grain size, carbide distribution, and carbide fraction were checked to identify any significant difference between images. A consistent microstructure for different samples in each group was desired in the experiment. After consistency examination, one sample was selected for SEM analysis. The selected sample should reveal clear microstructure and be etched properly to get high-quality images by SEM examination Microstructure examination by scanning electron microscope (SEM) SEM is a stronger technique than optical microscopy to examine the microstructure, since it produces images with higher magnification and higher resolution. Images taken by SEM make it possible to observe the phase changes in detail and collect data accurately. In the examination process, three magnifications, 1000X, 3300X and 10000X, were selected to observe the microstructures at different levels. The images taken at 1000X are better for an overall view and the images taken at 10000X are clear enough to observe characteristic structures of each grain, while 3300X images provide a balance between an overall view of the whole microstructure and high resolution.
41 26 To make sure the data from images are representative for statistical analysis, three images were taken in different areas under each magnification. The areas were selected randomly Data collection from SEM images To a certain extent, the microstructure changes under different heat treatments can be visible to the naked eye. In this project, we also wanted to make a rigorous statistical analysis to indicate how the microstructure changes under different heat treatments. Therefore, every feature of the steel microstructure should be quantified and a large amount of data should be collected from the SEM images. The size and location of each carbide grain are recorded in the data collecting process. From the raw data, we can get the average carbide size, carbides fraction, carbides count and interparticle spacing. The results from data collection help us to correlate the microstructures to mechanical properties and compare the different heat treatments. 4.3 PROCEDURES OF EDGED BLADE PERFORMANCE TESTS Introduction No matter how the heat treatment is applied or how the microstructure looks, the primary goal is achieving excellent mechanical properties for a knife blade. Therefore, a proper mechanical testing design will play an important role in this project.
42 27 Avoiding noise factors is the key point in the testing design. Many factors could be noisy in mechanical testing, such as operator, time, temperature and testing order. All factors were kept as consistent as possible in the mechanical testing. If there were factors that could not be controlled, a statistical method was applied to examine how these factors affect testing results. Based on the mechanical properties we want to study, four tests are designed in this project. Hardness: Rockwell Hardness C test (25 tests/heat treatment) Toughness: 3-point bend test, Impact test (5 tests/heat treatment) Edge retention: CATRA test (5 tests/heat treatment) Procedures Rockwell Hardness C Test Hardness is the most common and fundamental mechanical test for steels. In this project, the Rockwell Hardness C test is applied, since it s easy to use, accurate and standard. The tester measures the hardness by measuring the resistance to penetration of an indenter . There are also different scales that are determined by the indenter used and the load applied. The C scale is generally used in tool steel and stainless steel. A diamond with a cone angle of 120 and 150-kg load is used for C scale. The hardness number is given by Equation 1 . Where, t is the indentation depth ( mm ).
43 28 HRC t (1) The Rockwell Hardness tester used in this project is illustrated in Figure 6. Figure 6. Rockwell hardness tester Figure 7. Five hardness readings Five test samples with the same dimensions were tested for each group. Five readings were collected for each sample in different positions. The spacing of
44 29 these measure positions is compliant with ASTM E18-14a. The distance between the centers of two positions is larger than 3 times the diameter d (1.5 mm ) of the indenter, and the distance from the center of any position to an edge of the sample is larger than 2.5 times the diameter d of the indenter . Also, the five testing positions are kept consistent in all samples (shown in Figure 7). All tests were completed by two operators in one day. Both operator order and sample order were randomized. After data collection, a statistical method was used to examine whether the operator affected the testing results. There is no significant operator difference shown in the ANOVA table (see Table 18 in Appendix 4) Impact test: Toughness is a mechanical property that measures the ability of the material to resist fracture. An impact test is applied to measure this ability by measuring the energy absorbed during the fracture. Generally, a pendulum striker falls from a fixed height and the sample is fixed at the lowest point of the path. After breaking the sample, the striker goes back to a specific height that will be calculated and converted into the absorbed energy. Charpy U and V tests are widely used. The standard sample dimensions are the same in both Chapy U and V tests, however they require different shapes of notches.
45 30 When measuring smaller sample like knife blade material in this project, the Charpy U and V tests are not sensitive enough . An alternative impact test was developed. The testing machine is shown in Figure 8. Figure 8. Impact test machine As Figure 8 shows, a hammer with the weight of 11.5 lbs was set at a fixed height, 16 inch. The specimen was fixed at the bottom of the machine. Beside the specimen, a detector was placed to measure the impulse energy. Temperature is also an important factor affecting the toughness performance. To avoid the noise from different temperatures, all of the impact tests were completed in one day.
46 31 For the first run of this test, there was no specimen fixed at the bottom. The hammer was dropped from a height of 16 inches. The impulse energy of free drop was measured. Then, five samples with the same dimensions for each group were tested in random order. The detector collected the impulse energy data. Finally, the absorbed energy was calculated as the difference between impulse energy of each run and the free drop energy Point bend test The 3-Point bend test is a kind of failure strength test. A transverse force is applied on a sample until failure. In this type of test, the samples are usually rectangular in shape and the detailed dimensions are not standard. The test machine is illustrated in Figure 9. Figure 9. 3-Point Bend test machine As Figure 9 shows, there are three contact points made by cylinders during the test. Point 1 contacts the middle of the specimen to provide a pressure load. Point 2 and Point 3 support the specimen at the ends. In the test, the load is
47 32 increased at a constant rate, the maximum load and the bend distance are recorded when the specimen fails. In this project, five samples for each group were tested by the 3-Point bend test in a random order. Each of the samples was prepared in a standard size that had a thickness of 0.1 inch and a width of 0.7 inch. As for the test machine, it was also kept consistent during the test process. Therefore, all factors were fixed. The max load data is used to analyze the transverse failure performance CATRA test High cutting edge stability is a characteristic performance of CPM-M4 steel. The CATRA test was developed to quantify this property. The CATRA test machine is shown in Figure 10. Figure 10. CATRA test machine
48 33 In the test, a fixed load was applied on the sharpened samples. The CATRA machine cycled the cutting edge a fixed distance horizontally. Abrasive paper was selected as the test media and the depth of cut for each cycle was measured to quantify the cutting property of samples. At least 20 cycles were repeated for each sample. If the final cut depth is larger than 10mm in the 20 cycles, the test would be repeated until the final cut depth is less than 10mm. To quantify the cutting properties of different samples, the sum of the first three cycles defines the initial cutting performance and the sum of first 20 cycles defines the cutting edge retention. For consistency, all samples were prepared in a standard size and a standard sharpening process was applied on all samples. However, there are also many potential noise factors in the test. To avoid these factors, the test order was executed in five replications. There was one sample from each of the five heat treatments in each replication. For each replication, a same batch of abrasive paper was used and the tests were finished in one day. For the first three replications, the abrasive paper are from the same batch. A new batch of paper was used for the last two replications.
49 34 5 RESULTS 5.1 MICROSTRUCTURE: In this study, although different heat treating parameters are used, the general microstructure of CPM-M4 steel is tempered-martensite with carbides of varying composition. As Figure 11 shows, the spherical carbides are distributed uniformly in the matrix. Due to the PM process, the carbide size is fine and uniform. Figure 11. Optical microstructure of CPM-M4 steel, austenitized at 2100 F, tempered at 1025 F, magnification is 500X Based on the element analysis results from the EDX analysis and the typical features of different phases, an SEM image with phase identification is shown in Figure 12. MC and C M 6 are two major kinds of carbides distributed in the tempered-martensite matrix [16,17]. By EDX examination, the darker
50 35 MC carbides in the SEM image are vanadium-rich carbides. MC carbides usually appear spherical in shape and are distributed inside the matrix grains. On the other hand, the brighter C M 6 carbides are molybdenum and tungsten-rich carbides. Molybdenum and tungsten contents are much higher than vanadium and chromium contents for these carbides. The EDX results are shown in Figure 13. In other steel alloy microstructures, vanadium carbides are usually small in size compared to other carbides. However, in this study, these two kinds of carbides do not show a large difference in their size. Powder metallurgy is the major reason for the lack of difference because it makes all of the carbides fine and uniform in size. As a result, the other carbides, such as the MC carbides. C M 6 carbides, have a size similar to the vanadium-rich Figure 12. Phase identification of CPM-M4 steel, autenitized at 2200 F, tempered at 925 F